At the tomb of the unknown endodontist, there is a plaque that reads "Root canal
treatment is ... adhesive dentistry that are important and unique to endodontics.
Adhesive Dentistry and Endodontics: Materials, Clinical Strategies and Procedures for Restoration of Access Cavities: A Review Richard S. Schwartz, DDS, and Ron Fransman, DDS AbstraCI
The complexity of restorative dentistry has increased greatly in recent years, with the myriad of products used in "adhesive dentistry." So too has the "simple" matter of restoring access cavities after completion of endodontic treatment. This review discusses current methods of "bonding" to tooth structure, ceramic materials, and metals, with emphasis on those aspects that are important to endodontics. Specific materials, procedures and major decision making elements are discussed, as well as how. to avoid problems in compatibility between endodontic and restorative materials. Kev Words
Access cavities, adhesive dentistry, endodontics, restorative dentistry
Dr. Schwartz runs a private practice limited to Endodontics, and is Clinical Assistant Professor, UT Health Science Center at San Antonio, San Antonio, TX. Dr. Fransman runs a private practice limited to Endodontics, Amsterdam, Netherlands. Address requests for reprints to Dr. Schwartz, San Antonio, TX 78257; E-mail: [email protected]
Copyright © 2005 by the American Endodontists
At treatment the tomb isof not the complete unknown
endodontist, there a plaque that reads "Rootarticle canal until the tooth has isbeen restored." A recent reviewed the overall topic of restoration of endodontically treated teeth (1). This review \vill address in detail the important issues when restoring access cavities through natural tooth structure and restorative materials \vith emphasis on major decision making elements, material selection and clinical procedures. It will focus on those aspects of adhesive dentistry that are important and unique to endodontics. Contamination
of the Root Canal System
One of the primary goals of root canal treatment is to eliminate bacteria from the root canal system to the greatest possible extent (2, 3). Bacteria have been shown to be the etiology for apical periodontitis (4) and to be the cause of endodontic failure (2, 3, 5). One of the goals in restoring of the tooth after root canal treatment should be to prevent recontamination of the root canal system. Gross contamination can occur during the restorative process from poor isolation or poor aseptic technique. Contamination can also occur from loss of a temporary restoration or if leakage occurs. The same things can occur with a "permanent" restoration, but "permanent" materials tend to leak less than temporary materials (6). Exposure of gutta-percha to saliva in the pulp chamber results in migration of bacteria to the apex in a matter of days (2, 7-9). Endotoxin reaches the apex even faster (10). The importance of the coronal restoration in successful endodontic outcomes is widely accepted and has been supported by studies by Ray and Trope (11), Hommez et al. (12), Tronstad et al. (13), Iqbal et al. (14), and Siqueira et al. (2). However, studies by Riccuci et al. (15), Ricucci and Bergenholz (16), Heling et al. (17), and Malone et al. (18) indicate that contamination may not as important a factor in failure as is commonly believed. Therefore, it must be concluded that the significance of bacterial contamination as a cause of endodontic failure is not fully understood. Because there is clearly no benefit to introducing bacterial contamination into the root canal system, and since it may be a contributing factor in endodontic failure, a basic premise of this review \vill be that every effort should be made to prevent contamination. Temporization To minimize the likelihood of contamination, immediate restoration is recommended upon completion of root canal treatment (19-21). When immediate restoration is not possible, and the tooth must be temporized, a thick layer of temporary material should be used, preferably filling the whole chamber. The majority of restorative dentists prefer a cotton pellet in the chamber, however (22). If a cotton pellet or sponge is to be use, orifice barriers are recommended, to provide a second layer of protection against contamination in addition to the temporary material at the occlusal surface. Recommended procedure for placing orifice barriers: 1. Countersink the orifice with a round bur. 2. Clean the orifices and floor of the pulp chamber thoroughly \vith alcohol or a detergent to remove excess cement and debris. Air abrasion provides a dentin surface that is free of films and debris. 3. Place a temporary or "permanent" restorative material in the orifices and over the floor of the chamber.
Volume 31, Number 3, March 2005
Restoration of Access Cavities
Raview A bonded material such as composite resin or glass ionomer cement is preferred (23-27). Temporary materials may also be used (28). Mineral trioxide aggregate (MTA) may also be used (29). There is probably some benefit to using a material that is clear so that the restorative dentist can see the underlying obturating material if re-entry is needed into the canal system (1) (Fig. 1). Results varied in studies that evaluated temporary materials for the access cavities (21, 30-36). The most common materials tested were zinc oxide eugenol (such as IRM, Dentsply Int.), zinc oxide/calcium sulfate (Cavit, Premier Corp.) or resin based materials including composite resin and resin modified glass ionomer materials. Generally, all of the temporary materials were adequate if placed in a thickness of 3 mm or greater (21, 33-36). All temporary materials leak to some extent (20, 21, 37-40). The zinc oxide/calcium 'Sulfate materials are more resistant to microleakage than the zinc oxide eugenol materials (21, 34), probably because of setting expansion and water sorption (33). Although the zinc oxide
eugenol materials tend to leak more, they possess antimicrobial properties, making them more resistant to bacterial penetration (21, 34, 41). Both materials are simple to use. One study reported less leakage with the use of two materials in combination (42). Resin based temporary materials must be bonded to provide an effective seal, because they undergo polymerization shrinkage of 1 to 3% (30, 43). This is offset somewhat by the fact that they swell as they absorb water (30). Generally, bonded resin materials provide the best initial seal, but lack antimicrobial properties (30). They require more steps and more time to place than materials such as lRM or Cavit. Bonded resins are recommended for temporization that is likely to last more than 2 to 3 wk (42,44). Resin modified glass ionomer materials are also a good choice for long term temporization, because they provide a bond to dentin and enamel, and many have antimicrobial properties (44). Teeth requiring temporary post/crowns are a particular challenge, because of the difficulty in obtaining a good seal (45,46). To minimize
Figure 1. (A) Thepulp chamber has been thoroughlycleaned. (B) There was 37% phosphoric acid applied to the orificesand floor of the chamberfor 15 s. (C)The floor and orifices are sealedwith unfilled resin. (CourtesyofDr. Fred Barnett, Philadelphia.)
Schwartz and Fransman
Volume 3 t. Number 3. March 2005
1 the chances of contamination of the obturating material, a barrier may be placed over it with a seU-curing material. The post space should be restored as soon as possible and it may be beneficial to flush the post space with an antimicrobial irrigant when the temporary post is removed.
specific challenges which require specific strategies and materials. Often the access opening is prepared through two or three different substrates. The structural integrity of the tooth may also influence the choice of restorative materials. Each substrate will be addressed separately.
Restoring Access Openings When an access opening is made through an existing restoration, several things should be considered. Removal of all existing restorations is desirable if possible, because it allows more complete assessment for the presence of cracks and caries (47). This is particularly recommended for old class I and class 2 restorations, because they are likely to be removed later anyway, in the process of preparing the tooth for a crown. Magnification and caries detector are helpful in identifying cracks and for complete removal of caries (48). If the existing restoration is a crown or onlay that appears to be clinically satisfactory and replacement is not planned, the chamber and internal restorative materials should be examined carefully with magnification. Caries detector should be painted on the internal tooth surfaces. Any areas stained by the caries detector, particularly adjacent to restorations, should be examined carefully for softness or gaps (Fig. 2). Caries detector may also stain sound areas of dentin that have decreased mineral content (49). The key to the presence of caries is determined by whether the stained areas are hard or soft. Many times caries can be "identified internally, necessitating replacement of the crown. Access openings made through an existing restoration results in loss of retention (50-52) and strength (53). When the access opening is restored, loss of retention is reversed (51, 52). If a post is added, additional retention is gained (51). Ideally, we would like to restore access cavities with a restorative material that provides a permanent, leak proof seal. Unfortunately, no such material is available. All materials that we use and restorations that we place leak to some extent. This includes intracoronal restorations including bonded resin and glass ionomer materials (38, 54) as well as the metal or ceramic extra-coronal restorations (55, 56). To minimize leakage, bonded restorations are recommended, regardless of the restorative material (6, 57). Access openings are made through a number of different restorative materials, including gold alloys, base metal alloys and porcelain, as well as enamel and dentin. Bonding to each of these substrates present
Bonding to Enamel Enamel is often present along the margins of access preparations of anterior teeth. The resin bond to etched enamel is strong and durable. The technique dates back to 1955 (58). Etching of enamel with an acid such as 30 to 40% phosphoric acid results in selective dissolution of the enamel prisms and creates a surface \vith a high surface energy that allows effective wetting by a low viscosity resin. Microporosities are created within and around the enamel prisms that can be infiltrated with resin and polymerized in-situ (59). These "resin tags" provide micromechanical retention. Bond strengths are typically in the range of 20 megapascals (Mpa) (60). Megapascals are a measure of the force per unit area that is required to break the bond. Self-etching adhesive systems, which \vill be discussed in the section on bonding to dentin, etch ground enamel fairly well, but do not etch unground, aprismatic enamel effectively (61-63). Therefore, enamel margins should be beveled when using self-etching adhesive systems. It is critical to prevent contamination of etched enamel with blood, saliva or moisture (64). Poorly etched enamel leads to staining at the margins of the restoration (65). A good enamel bond protects the underlying dentin bond which is less durable (66).
Bonding to Metal-Ceramic and All-Ceramic Restorations Access cavities are often made through metal-ceramic or all-ceramic materials, so attaining an effective, durable bond is important when restoring them. The literature is unambiguous that the best method to bond to porcelain is to first roughen the surface by acid etching and then apply a silane coupling agent, followed by the resin (67-70), Bond strengths of 13 to 17 Mpa have been reported, and failure is often cohesive within the porcelain, meaning that the interfacial bond strength exceeds the strength of the porcelain itself (71-73) . Bonding to porcelain was initially developed as a method for repair of fractured metal-ceramic crowns. Improvements in the technique allowed porcelain veneers to become a common clinical procedure. Etched ceramic materials form a strong, durable bond \vith resin (74). Micro mechanical bonding can be attained by roughening the porcelain with a bur, air-abrasion or etching with hydrofluoric acid. However, acid etching is the most effective method (73, 75, 76). The first to introduce acid etching of porcelain was Calamia in 1983 (77). Adhesion between the resin and porcelain may be enhanced by the use of a silane-coupling agent. Silane acts as a surfactant to lower surface tension and forms double bonds with OH groups in the porcelain, forming a siloxane bond. At the other end of the silane molecule is a methacrylate group that copolymerizes \vith resin. The use of a silanecoupling agent \vith porcelain was first described by Rochette in 1975
Cariesdetectorwas applied to the inside of an access cavity.Notehow the caries detector accentuates the caries under the compositebuildup. (Courtesyof Dr. GaryCarr, San Diego.)
Volume 3t, ~umber
3, March 2005
Hydrofluoric acid provides greater surface roughness to porcelain than air abrasion or roughening \>ith a bur (75). It works by dissolving the glass particles (leu cite) within the porcelain (Fig. 3). Most of the porcelains used in metal-ceramic restorations are feldspathic porcelains that contain leucite. Some ceramic materials, such as low fusing porcelains, do not contain leucite and are not etched effectively by
Restoration of Access Cmities
Figure 3. SEM of etched porcelain. (Courtesy ofDr. Bart VanMeerbeek, Leuven,
Belgium.) Figure 4. Most restorative composites are too translucent
hydrofluoric acid (79). However, hydrofluoric acid is effective with most of the current ceramic restorative materials (80-83). Hydrofluoric acid is usually provided in a 10% concentration in a syringe. It is very important to follow the manufacturer's instructions, as an application time that is too short will produce an inadequate etch, while an application time that is too long may render the porcelain brittle and thus more prone to fracture (84).
(gray) to provide a
good match when restoring access cavities in metal-ceramic crowns.
are composite resins that contain opaquers. They may be covered with more translucent composite materials. Several composites are available that are quite opaque and work well when restoting access cavities in metal-ceramic crowns. Composite stains can be used to accentuate pits and fissures to further enhance the cosmetic result (Fig. 5).
Silane acts as a "coupling agent" enhancing the bond between the resin and ceramic materials. It is supplied premixed or as a two bottle system that is mixed at the time of use. It is applied to the etched surface and must be thoroughly air dried (85). A low viscosity resin adhesive is then flowed over the surface and polymerized. Once again, it is very important to follow the manufacturer's instructions. Silane has a limited shelf life. Storage in the refrigerator will extend its useful life, but it should be used at room temperature (86). The two bottle silanes have the longest shelf life (7 I). Silane that is past the expiration date or that contains precipitates should be discarded (86). Air Abrasion
Bonding to Metal
The metal portion of metal-ceramic crowns is not usually significant when restoring access openings, so no e.-ilraprocedures are necessary to deal ,vith it. However, for crowns in which all or part of the occlusal surface is metal, adhesion may be desirable. Adhesion to metal is generally obtained by mechanical means. Surface roughness may be created with a bur or air abrasion, which provides micromechanical retention (89). Chemical adhesion is also possible ,vith metals that form an oxide layer (90). Silane has no effect on bonding to metal (9 I) . Several studies have shown tin plating of metal enhances mechanical retention (92-96). Chromium plating also works well (96). Plating devices are available that can be used intraorally. Although effective, this
Air abrasion is sometimes recommended to clean the porcelain and provide surface roughness. Several companies sell "micro-etchers" that can be used chairside. Aluminum oxide particles are sprayed onto the surface at about 80 psi. Fiftymicron particles have been shown to produce a more retentive surface than 100 /lm particles (87). Two studies reported that air abrasion has a negligible effect on bond strength, however (76, 88). Etching and application of silane are the two most important steps. CosmeUcs
When restoting the access cavity of a ceramic crown, it is often a challenge to produce a good cosmetic result. Many times it is difficult to mask the underlying metal of a metal-ceramic crown. This is particularly true if the porcelain is thin. It is not uncommon to see the metal showing through the composite. The second challenge is to match the optical properties of the porcelain. This is true for metal-ceramic crowns as well as all-ceramic crowns. Most composites are too low in value (too gray and translucent) to effectively match the surrounding porcelain (Fig. 4). Several products are available that may be used to mask the underlying metal before the restorative composite is placed. Most of these
Schwanz and Fransman
Figure 5. With knowledge of color, translucency and occlusal anatomy, beau-
tiful results are achievable when restoring access cavities with composite resins.
Volume 31, Number 3, March 200;
procedure has never gained popularity. Meta! primers are an alternative that enhances the bond between metal and resin. They have been shown to be effective and do not require any special equipment (97-99).
Bonding to Dentin: Resin Materials
Bonding to dentin with resin materials is more complex than bonding to en:unel or porcelain. Dentin consists of approximately 50% inorganic mineral (hydroxyapatite) by volume, 30% organic components (primarily type 1 collagen) and 20% fluid (100). The wet environment and relative lack of a mineralized surface made it a challenge to develop materials that bond to dentin. Current strategies for dentin adhesion were first described by Nakabayashi in 1982 (101), but his ideas were not widely accepted for a number of years. Nakabayashi showed that resin bonding to dentin could be obtained by applying an acid to expose the collagen matrix and dentinal tubules, applying a hydrophilic ("water loving") resin material to the demineralized surface and polymerizing the resin in situ. The collagen matrix and dentin tubules, to a lesser extent, provide mechanical retention for the resin. Although not as durable and reliable as en:unel bonding, steady improvements have been made in dentin bonding and in simplifying dentin-bonding procedures. Most in vitro studies of dentin bonding report on bond strengths, microleakage, or both. like en:unel, bond strengths are usually reported in Mpa. Depending on the test method used, initial bond strengths can be obtained that are equal or greater to those of etched en:unel. However, dentin bonding is not as durable as en:unel bonding or as stable. It is well documented that bond strengths decrease with time and function. This has been shown in vitro (66, 102-109) and in vivo (110, 111). Microleakage is probably a more important issue to endodontics than bond strength. None of the current adhesive systems are capable of preventing microleakage over the long term (65, 112117). There is not a direct relationship between bond strength and microleakage (116). Dentin adhesive systems utilize an acid as the first step of the bonding process to remove or penetrate through the smear layer and demineralize the dentin surface. The smear layer covers the surface of ground dentin and consists of ground up collagen, hydroxyapatite, bacteria, and salivary components (59). Most dentin adhesive systems can be categorized as "etch and rinse" or "self etching," based on the acid etching process (59).
Figure 6. SEM of a demineralizedspecimen showingresin penetration into the hybrid layer and dentinaltubules. (CourtesyofDr. Bart VanMeerbeek,Leuven, Belgium.)
residual carrier/solvent is left behind (119), which makes the bond more subject to hydrolytic breakdown (119). "Sell Etching" Adhesives
Most of the "self etching" products combine an acid with the primer. Rather than removing the smear layer, they penetrate through it and incorporate it into the "hybrid layer." The acidic primer is applied to the dentin surface and dried with a stre:un of air. There is no rinsing step. A resin adhesive is then applied and polymerized, followed by the restorative material. The "self etching" systems can be categorizes as "strong" or "aggressive" (pH 2) (59, 120, 121). The strong "self etching" systems form a hybrid layer of approximately 5 JLm in thickness, similar to phosphoric acid, whereas the mild systems form a hybrid layer of about 1 JLmicron (120, 121). There does not appear to be clinical significance to this difference in thickness, however (121). The "strong" systems generally produce a superior bond to en:unel than the "weak" systems (59), particularly with unground en:unel (61-63). Dentin Adhesive "Generations"
"Etch and Rinse" Adhesives
Most of the "etch and rinse" adhesive systems utilize a strong acid such as 30 to 40% phosphoric acid. When phosphoric acid is applied to dentin, the surface is demineralized to a depth of about 5 JLm. The acid is rinsed offafter about 15 s, removing the smear layer and exposing the collagen matrix and network of dentinal tubules for resin bonding. A hydrophilic primer is then applied to the surface to infiltrate the collagen matrix and tubules. The primer contains a resinous material in a volatile carrier/solvent, such as alcohol or acetone, which carries the resinous material into the collagen matrix and dentinal tubules. The surface must be wet (moist) for the primer to penetrate effectively.After the primer is in place a stre:un of air is used to evaporate the carrier and leave the resin behind. A hydrophobic ("water hating") resin monomer (adhesive) is then applied and polymerized, which adheres to the infiltrated resin from the primer. A "hybrid layer" or "interdiffusion zone" is formed that consists of resin, collagen and hydroxyapatite crystals (59) (Fig. 6). It bonds the hydrophobic restorative materials to the underlying hydrophilic dentin. Poor bond strengths and increased microleakage result from excessive etching (118). The s:une is true if
Many of the "etch and rinse" adhesive systems require three steps (etch, primer, adhesive), and are known as "4th generation" adhesive systems. The "generation" of a dentin adhesive generally follows the order in which they were developed and each "generation" utilizes different bonding procedures. The "5th generation" adhesive systems are "etch and rinse," followed by application of a combined primer and adhesive. These are sometimes referred to "single bottle" adhesive systems. Some require several applications of the primer/adhesive, however. The "6th generation" adhesives utilize an acidic ("self etching") primer followed by an adhesive. The 5th and 6th generations are generally two step procedures, while the 7th generation combines everything (acid, primer and adhesive) into one step. Many of the "self etching" products require fewer steps and less time than the "etch and rinse" products, and are considered to be less "technique sensitive" (59). There are still a number of questions about them, however, such as the unknown effects of incorporating partially dissolved hydroxyapatite crystals and smear layer into the hybrid layer. There is also the question of how much of the carrier/solvent remains behind. Because they are relatively new, there are currently no long-term
II JOE -
Volume 31, Number 3, March 2005
Restoration of Access Cavities
.r " a!,
clinical studies with the "self etching" adhesive systems. The three step
the order of 8 Mpa. But unlike resins, they form a "dynamic" bond. As
adhesive systems genernlly perronn
better in in vitro testing than the adhe-
sive systems that combine steps (59, 65, 66, 107, 121, 122), although the differences lessen with time as the bonds degrade (66, 107). The "self etching" adhesive systems are also less effectivethan the "etch and rinse" systems when bonding to sclerotic dentin and caries effected dentin (123, 124). They also have compatibility problems with some composite restorative materials, which will be discussed in the section on self-cure and dual-cure composites. The single step (7th generation) adhesives are a fairly recent addition to the market. Atthis point in their development, they produce consistentlylower bond strengths in vitro than the others (59, 107, 121, 125) and are not compatible with self-cure or dual-cure composites (126). Most of the current research is directed toward improving the performance ofthe simplifiedadhesive systems,and theywill probably continue to improve. Some of the common acronyms used in resin bonding are shown in Table 1. Examples of commercial dentin bonding systems are shown in Table 2. Wet Bonding
Most adhesive systems utilize "wet bonding." If the etched dentin surface is dried excessively, the collagen matrix collapses and prevents effective infiltration of the primer. The result is low bond strengths and excessive microleakage (127-129). Excessive moisture has similar negative effects on adhesion (128, 129). An effective method to provide the proper amount of moisture is to dry the surface thoroughly and then rewet it with a moist sponge, so that the surface is damp, but there is no visible pooling (127, 130). ; Bonding 10 Denlin: Tradilional
Glass ionomer cements are made primarily of alumina, silica and polyalkenoic acid and are self curing materials. Most glass ionomer cements release fluoride for a period of time after initial placement. They are the only restorative materials that depend primarily on a chemical bond to tooth structure (131). They form an ionic bond to the hydroxyapatite at the dentin surface (132) and also obtain mechanical retention from microporosities in the hydroxyapatite (133). Glass ionomer materials form lower initial bond strengths to dentin than resins, on
bonds are broken,
one of the factors that allow glass ionomer cements to succeed clinically, despite relatively low bond strengths. Other factors are low polymerization shrinkage and a coefficient of thermal expansion that is similar to tooth structure. Some glass ionomer materials also possess antimicrobial properties (134 -136) . When placing glass ionomer cements, the surface is cleaned and then treated with a weak acid such as polymaleic acid (131). The acid removes debris from the dentin surface, removes the smear layer, and exposes hydroxyapatite crystals. It creates microporosities in the hydroxyapatite for mechanical retention, but there is minimal dissolution (131, 133). Because glass ionomer cements rely on ionic bonding to the hydroxyapatite, strong acids should be avoided because they cause almost total elimination of mineral from the dentin surface (137). Traditional glass ionomer cements are not widely used for clinical procedures because they set slowly and must be protected from moisture and dehydration during the setting reaction, which in many cases is not complete for 24 h. They are also relativelyweak and generally not as esthetic as other restorative materials. Bonding 10 Denlin: Resin Modified Glass lonomer Malerials Resin modified glass ionomer (RMGI) materials were developed to overcome some of the undesirable properties of the traditional glass ionomer cements. RMGI materials contain glass ionomer cement to which a light-cure resin is added. The purpose of the resin is to allow immediate light polymerization after the material is placed. The resin also protects the glass ionomer cement from dehydration, and improves the physical and mechanical characteristics and optical properties. True RMGImaterials utilize similar bonding procedures as glass ionomer cements and do not require a dentin-bonding agent. Endodonlic Issues in Denlin Bonding Some of the materials used in endodontics may have a significant impact on the bonding process. These issues apply not only to restora-
Commonabbreviationsused in dental adhesive literature
Bisphenol glycidyl methacrylate Ethylenediaminetetracitic acid
Unfilled resin-The original Chelating agent sometimes demineralize the dentin
MMA NPG-GMA PMDM TEG-DMA UDMA
Methyl methacrylate N-Phenylglycine glycidyl methacrylate Pyromellitic acid dimdiethylmethacrylate Triethylene glycol dimethacrylate Urethane dimethacrylate
Low viscosity hydrophilic acrylic monomer used in dentin adhesive systems Low viscosity acrylic monomer used in dentin adhesives. Also used for metal bonding Basic acrylic molecule Low viscosity hydrophilic acrylic monomer used in dentin adhesives Low viscosity hydrophilic acrylic monomer used in dentin adhesives Low viscosity hydrophilic acrylic monomer used in dentin adhesives Unfilled resin. Alternative composite matrix material for composites. Sometimes combined with Bis-GMA
acrylic matrix material in composite resins used to remove the smear layer and
OptiBond Total Etch Scotch bond Multipurpose One Step Prime&Bond Clearfil SE OptiBond Solo SE Prompt L-Pop 2 I-Bond
Schwartz and Fransman
Three step, etch and rinse, "4 generation" Three step, etch and rinse, "4th generation" Three step, etch and rinse, "4th generation" Two step, "single bottle," etch and rinse, "5th generation" Two step, "single bottle," etch and rinse, "5th generation" Two step, self-etching, "6th generation" Two step, self-etching, "6th generation" One step, self-etching, "7th generation" One step, self-etching, "7th generation"
3M Bisco Dentsply Kuraray Kerr 3 M/ESPE Kulzer
but new bonds form. This is
Volume 31, Number 3, March 2005
Review d.As his is :lini-
!ion of access cavities, but also to the obturating adhesive article.
materials that utilize
which will be discussed
These are particularly
In endodontics, sealers
reverse the effects of the sodium hypochlorite.
is one of many sub-
stances that can prevent or stop the polymerization
(138) and can interfere with bonding (139). If resin bonding is planned
ical steps are needed to minimize
to remove visible signs of
eugenol or not,
leave behind an oily layer of debris that must be removed
(140, 141). Air abrasion
cleaning the dentin surface
be etched with an acid, such as phosphoric
(Fig. 7). Once it is clean, the dentin should
the dentin surface
acid and then rinsed.
to a depth
rich layer. Several studies
"total etch" (three step) procedure contaminated
is an effective method
the effects of the eugenol. The surface
allows effective bonding
the "self etching"
it. Eugenol has no effect on glass ionomer
of its antimicrobial
tion of bacterial
It has oxidative and causes
in cellular actions
that cause deactiva-
gained a following as an irrigating strengths sodium
exhibits resin bond strengths
that are significantly
(145-149). One study reported bond as low as 8.5 Mpa (147). Increased microleakage was also (150). This phenomenon probably occurs because sodium
is an oxidizing agent, which leaves behind an oxygen rich
layer on the dentin surface. Oxygen is another
the effects of sodium
used in endodontics
silver amalgam alloy is the most common
with few steps, and provides
is often recommended
(57) in which a resin adhe-
on the cavity walls before condensation
sive is placed
(161). The clinical tech-
alloy. The adhesive provides an immediate
of the amalgam
seal. When amalgam alloy is
form at the amalgam
or other restorative
alloy, that offers theoretical
interface with tooth structure
(162). One strategy to use with amalgam
is to seal only the chamber
and orifices with adhesive resin to provide initial protection
of the root
canal system from contamination.
With time the amalgam
\vill corrode at the other interfacial more durable than resin.
areas and provide a seal that may be
. There is a theoretical pure spherical
alloys have slight setting expansion,
(163), whereas spherical
to using ad-mixture
refers to a mixture
slightly while setting (163).
is likely to remain the
for the near future, and because
are used routinely
treated teeth, this issue will have to be addressed. products
access cavities in metal crowns
that inhibits the
levels. Lai et al. and Yiu et al. reported
results (149, 150). Because sodium hypochlorite primary
which tends to reduce
(147,155,156) or placement of resin-modified glass ionomer materials (157). Caries detector did not affect resin bond strengths (158, 159), but chloroform and halothane resulted in significant loss of bond strength (160).
acid (153, 154). No loss of
polymerization of resins (151). Morris et al. showed that application of 10% ascorbic acid or 10% sodium ascorbate, both of which are reducbond strengths
of adhesive resins because it has the same active ingredient
Several studies have shown that dentin that has been exposed sodium hypochlorite
used without an adhesive, it leaks initially, but "self seals" with time as
lipid and fatty acid degradation
Silver Amalgam Allov
used as an endodontic
(147, 148). Reduced bond strengths were shown after the use of RC prep (Premier) (146). Electro-chemically activated water has
Not surprisingly, Sodium hypochlorite
leaves behind an oxygen rich surface
have been tested for their effects on bonding. Not surprisingly,
the eugenol rich smear layer into the hybrid layer, rather than removing
that are applied to dentin during endodontic
(24, 142). An "etch and rinse" adhesive
system should be used, because
Applied to Dentin
for a dentin surface that is contaminated
sealer. Many temporary
timely issues for endodontics
should be cleaned with alcohol or a detergent
are widely used in
would also solve this problem. Sodium hypochlorite and EDTA have also been shown to reduce the tensile strength and microhardness of dentin
in a subsequent
Future adhesive a reducing
Not surprisingly, restoring be bonded provide
resin is the most common
access cavities in ceramic to tooth structure
and most restorative
a good match of color and surface
can also strengthen
ture, at least in the short term (164, 165). The limitations primarily reported
resin as a restorative
to exhibit shrinkage
on the adhesive
One study reported FIgure 1. Example of the cleaning effect of sandblasting.
Cleaning with alcohol and chloroform left a film on the dentin surface, shown in the first picture. Note how much cleaner the dentin appears in the second picture, after microabrasion (Courtesy ofDr. Fred Tsusui, Los Angeles).
Volume 31, Number 3, March 2005
in the range of 2 to 6% during polymer-
ization (43, 166). Less filler (such as found in "flowable" results in more shrinkage
(166, 167). Polymerization
bond that often results in gap formation
of dentinal gaps found in vivo was 14
to 54% of the total interface restorations
(168). Marginal deterioration of composite expedites the loss of dentin adhesion (169).
Composite self- (chemical)
cure or dual-cure.
come in several forms: light-cure, light-cure
i Ii Iii' 1"
consist of a
Restoration of Access Cavities
I I I I
Rgure 8. (A) The access cavityis clean and ready to restore. (B) There was 10%hydrofluoric acid applied to the porcelain for 1 min and then rinsed thorougWy. (C) Therewas37%phosphoric acid appliedto the dentinand porcelain for 15to 20 s. It demineralizesthedentinsurfaceand cleanstheporcelain. (D) Theporcelain
is thorougWyair dried and silane is applied and dried. single paste and polymerization is initiated with a curing light. Self-cure materials consist of two pastes that are mixed together to initiate polymerization. Dual-cure materials also consist of two pastes that are mixed together to initiate polymerization, but may also be light activated. Dual-cure materials havethe advantageof rapid polymeMuion in the areas iITadiatedbythe curing ligh~but chemical polymeMuion occurs in areas the lightcan not reach. Light-cure materials polymerize in a matter of seconds and generally have the best physical properties. However, they have several disadvantages. Because of the rapid polymerization, they tend to stress the adhesive bond to tooth structure more than the slower self-cure composites (I 67). The stress is sometimes so great that the restorative material debonds at the weakest interface (43, 170). For example, in class 5 composite restorations, they tend to debond
at the interface with cementum, which forms a weaker bond than enamel (54). Because most curing lights can only effectively polymerize a thickness of 2 to 3 mm of composite material, cavities must be filled incrementally, a time consuming and tedious task. An access cavity may require 3 to 5 increments. Because curing lights lose intensity with distance, the light intensity may be greatly reduced at the floor of the chamber when curing through an access opening in a crown. In addition, it may not be possible to irradiate all areas inside an access cavity because of undercuts or difficulty in obtaining the proper angle with the light. Self-cure materials may be bulk filled because they do not require penetration with a curing light. They polymerize more slowly than lightcure materials, allowing the material to flow during polymerization contraction, and placing less stress on the adhesive bond (43, 167). The
Schwartz and Fransman
Volume 3 t, Number 3. March 2005
(E) A dentin primer is applied to all internal surfaces and air dried, and a dentin adhesive is applied to all internal surfaces and light polymerized. (F) A tlowable composite is injected into the orifices and on the chamber tloor and polymerized. This method minimizes voids between the restorative Rgure 8 (conDnued).
material and dentin. Because it is somewhat translucent, it makes location the canals easier if re-entry is necessary at a later time. (G) Incremental build-up, light composite over dark. Increments should be only 2 to 3 mm in thickness to allow adequate polymerization. (H) Application of opaque composite. This is often necessary when restoring metal-ceramic crowns that tend to be quite opaque.
same is true for dual-cure
in the areas that are not irradiated
by the curing light. The problem access ration faces greater with
cavities because of a concept known as Cofactor or configufactor (43, 167). Cofactor refers to the ratio of bonded surto free or un bonded
the stress from polymerization Cofactor
Volume 31, Number 3, March 2005
The higher shrinkage considered
the Cofactor, (43).
to be at risk
and micro leakage
In a class
ratio might be 1: 1. In an access cavity, the Cofactor might be 6: 1 or even 10:1. In a root canal system obturated with a bonded resin material,
it might be 100:1
An incremental partially overcomes
sible because atmospheric the external
of Cofactor. Incremental
filling is pos-
oxygen prevents complete polymerization
surface of the resin. This oily surface is referred
to as the
Restoration of Access Cavities
Figure 8 (condnued). (I) Ocre colored modifiers are placed in the grooves. (J) Cuspinclinesand triangularridges are builtup. (K) Brownmodifiersare added to the groovesand occlusion is checked. (L) Final result.
"oxygen inhibited layer (I 51)." Because of the unpolymerized surface layer, additional increments may be added and polymerized and a strong chemical bond is formed between increments (I 51). Incremental filling allows complete polymerization of each increment, and lessens the stress from polymerization shrinkage 172) because the Cofactoris more favorable for each increment than if the cavitywas bulk filled. Another strategy to lessen the effects of Cofactor is to use slow setting self-cured materials that flow during polymerization, thus reducing stress (31, 167). If contamination occurs with blood or saliva during incremental filling, the bond between increments may be ruined. However, if the surface is rinsed, dried and a dentin adhesive is applied, there is no loss of bond strength (I 73).
Schwartz and Fransman
mass Ionomer cemenr _
Resin ModIied mass kInomer MateItaIs
Both types of glass ionomer materials may be bulk filled. Most of the RMGImaterials are dual-cure. Traditional glass ionomer cements are selfcure and haveverylittlepolymerization shrinkage. Because resin is added to RMGImaterials, they exhibit some polymerization shrinkage, although less than composite resins. Both types of glass ionomer materials are useful for bulk filling access cavities. Even though they bond to tooth structure, the bond strengths are too low to provide significantstrengthening effect (174).
Maleriallncompalibililies The "self etching" adhesive systems have generally been shown to result in low bond strengths when used \vith self-cure composites and
Volume 31, Number 3, March 2005
-Review dual·cure composites that h:lI'e not been light activated (126, 175178). This is in part because of residual acid on the dentin surface. Self-cure composites contain tertiary amines in the catalyst that initiate the polymerization reaction and have a high pH. Loss of bond strength results because residual acid from the acidic primer inhibits the basic amines, resulting in incomplete polymerization at the interface between the adhesive and the restorative material (175, 176, 179, 180). Dualcure composites exhibit bond strengths comparable to light-cure composites in the areas that are effectively light-cured (177), because they are not dependent on the basic amines. One study reported lower bond strengths with the self-cure composites than light-cure composites with "etch and rinse," single bottle (Sth generation) adhesives as well (181). The second problem with many of the "self etching" adhesive systems is that they act as permeable membranes. This is a problem when they are used with restorative materials that polymerize slowly. A permeable adhesive layer allows penetration of moisture from the dentin to the interface with the restorative material, which is hydrophobic (122,179). Moisture penetration can result in a phenomenon known in pol~mer chemistry as "emulsion polymerization," in which there is poor adaptation between the adhesive and restorative material (122). Moisture at the interface probably also contributes to the degradation of the bond over time (122).
Clinical Strategies Most strategies for restoring access cavities require several steps and at least two layers of restorative material. Many approaches utilize an adhesive system and two restorative materials. The exception is unbonded amalgam alloy. Restoring Access Cavities with Tooth Colored Materials
tight-cure composite can be used to fill the entire access cavity if it is filled incrementally. Tllis method will provide the strongest bond to tooth structure (181) and is the preferred method when it is necessary to ma.ximize the tooth strengthening effects of the restoration. When executed with skill and knowledge of the materials, excellent esthetic results are possible (Fig. 8). However, this is a slow, time consuming method. High initial bond strengths are also obtained \vith dual-cure composites that are placed incrementally and light polymerized (177). This method may be preferred to incremental fillwith purely light-cured materials if there are concerns about light penetration to all areas of the cavity. As discussed earlier, the 4th generation adhesive systems are preferable for endodontic restorative applications with composite materials. They tend to form the best bond to dentin, and have few compatibility problems with restorative resins. They are also effective despite the use of eugenol containing sealers or temporary materials. A method to restore access cavities in teeth \vith ceramic restorations: tight-cure composite 1. Clean the internal surfaces with a brush or cotton pellet containing a solvent such as alcohol. 2. Sandblast the cavity, metal and ceramic, or liglllly refresh them \vith a bur. 3. Etch the ceramic \vith hydrofluoric acid or other appropriate etchant. 4. Rinse and dry. S. Applyphosphoric acid to the inside of the access cavity if restoring with composite. Etching with phosphoric acid adds no retention to porcelain, but it cleans the porcelain and enhances the silane adaptation (182). 6. Rinse and dry. 7. Apply silane agent to the porcelain and dry.
Volume 31, Number 3, March 200;
8. Applya dentin primer and adhesive to the internal walls and light cure. 9. Fill the cavity incrementally with no increments greater than 3 mm.
10. tight cure each increment for 40 s (time depends on type of light used) . 11. The restoration should be slightly overfilled so it can be finished back to the margins. 12. Contour and adjust the occlusion. 13. Finish and polish the restoration. In many cases, it is desirable to bulk fill most of the cavity with a glass ionomer material or self-cure or dual-cure composite, then veneer it \vith a light-cure composite material that is esthetic and will withstand occlusal function. This method is more efficient than using a purely light-cure composite, but the esthetic result may not be as good. A simple method to restore access cavities in teeth with ceramic restorations: Glass ionomer and composite 1. Treat the dentin with a polyalkenoic acid for 30 s. 2. Bulk fill,vith a dual-cure glass ionomer material to \,ithin 2 to 3 mm of the cavo-surface margin and light cure. 3. Etch the ceramic material with 10% hydrofluoric acid, or other suitable etching gel for 1 min, depending on the product. 4. Rinse and dry. 5. Apply silane to the etched ceramic surface and air dry. 6. Apply the dentin primer and adhesive to the glass ionomer material and etched ceramic and light cure. 7. Place the first increment of light-cure composite. The first increment should include the longest vertical wall and taper to the base of the opposing vertical wall. 8. tight cure for 40 s (time depends on type of light used). 9. Fill the remaining space \vith the second increment and light cure. The restoration should be slightly overfilled so it can be finished back to the margins. 10. Contour and adjust the occlusion. 11. Finish and polish the restoration. A Simple Procedure
II I I I I
The procedures are similar to those described \vith glass ionomer material, but a 4th generation dentin adhesive system is used on the dentin and a dual-cure composite is substituted for the glass ionomer material. 1. Treat the dentin and enamel, if present, with 30 to 40% phosphoric acid for 15 s. 2. ThorougWy rinse and dry the dentin then rewet ,vith a moist sponge. 3. Apply primer and adhesive, following the manufacturer's instructions. 4. Bulk fill with a dual-cure or self-cure composite to \vithin 2 to 3 mm of the cavo-surface margin and light cure. S. Etch the ceramic material with 10% hydrofluoric acid, or other suitable etching gel for 1 min. 6. Rinse and dry. 7. Apply silane to the etched ceramic surface and air dry. 8. Apply the dentin primer and adhesive to the etched ceranlic and light cure for 15 s. 9. Place the first increment of light-cure composite. The first increment should include the longest vertical wall and taper to the base of the opposing vertical wall. 10. tight cure for 40 s. 11. Fill the remaining space with the second increment and light cure.
Restoration of Access Ca~ities
I ik ••
12. Contour and adjust the occlusion. 13. Finish and polish the restoration. Dual-cure composites that are bulk filled develop relatively low bond strengths to dentin, comparable to glass ionomer materials. Resin adhesives lose bond strength with time and function, whereas glass ionomer bond strengths are relatively stable. So there is little if any benefit to the use of dual-cure composites over glass ionomer materials for bulk filling the cavity.
15. Ricucci D, Grondahl K, Bergenholtz G. Periapical status of root-filled teeth exposed to the oral environment by loss of restomtion or caries. Oral Surg Oral /tied Oral Pathol Oral Radiol Endod 2000;90:354-9. 16. Ricucd D, Bergenholtz G. Bacterial status in root-filled teeth exposed to the oral environment by loss of restomtion and fracture or caries: a histobacteriological
1, Bialla-Shenkman S, Turetzky A, HorwitzJ, Sela]. The outcome of teeth with
periapical periodontitis treated with nonsurgical endodontic tre-atment: a computerized morphometric
study. Quintessence Int 2001;32:39i-400.
18. Malone KH 3rd, Donnelly JC. An in vitro evaluation of coronal microleakage obtumted root canals without coronal restorations. J Endod 199i;23:35-S. failure caused by inadequate restomtive procedures: mendations. J Prosthet Dent 2002;8i:6i4-S.
1. Prevent contamination of the root canal system. 2. Restore access cavities immediately whenever possible. 3. Use bonded materials
6. "Self etching" adhesives should not be used with self-cure or dual-cure restorative composites. 7. When restoring access cavities, the best esthetics and highest initial strength is obtained with an incremental fill technique with composite resin. 8. A more efficient technique which provides acceptable esthetics is to bulk fillwith a glass ionomermaterial to\vithin 2 to 3 mm of the cavo-surface margin, followed by two increments of light-cure composite. 9. If retention of a crown or bridge abutment is a concern after root canal treatment, post placement increases retention to greater than the original.
2. Siqueira]F Jr, Rocas IN, Favieri A, Abad EC, Castro AJ, Gahyva SM. Bacterial leakage in coronally unsealed root canals obturated with 3 different techniques. Oral Med Oral Pathol Oral Radio! Endod 2000;90:64i-50 .
3. Siqueira]F Jr. Aetiology of root canal treatment failure and why well-treated can fail. Int EndodJ 2001;34:1-10. 4. Kakehashi S, Stanley HR, Fitzgerald R]. The effects of surgical exposures
rats. Oral Surg Oral Med Oral Path
22. Dillard CR, Barfield RD, Tilashalski KR, Chavers LS, Eleazer PD. Comparison endodontist versus generalist regarding preference for postendodontic ton pellets in pulp chamber. J Endod 2002;2S:656-i.
terial penetration of endodontically treated teeth coronally sealed with a dentin bonding agent. J Endod 2001;2i:354-i. terials used to create an intracoronal 2002;28:59-61.
seal in endodontically
of five ma-
treated teeth. J Endod
26. Belli S, Zhang Y, Pereim PN, Ozer F, Pashley DH. Regional bond strengths of adhesive resins to pulp chamber dentin. J Endod 2001;2i:52i-32.
Belli S, Zhang Y, Pereim PN, Pashley DII. Adhesive sealing of the pulp chamber. J Endod 2001;2i:521-6.
2S. Pisano DM, DiFiore PM, McClanahanSB, Lautenschlager EP, Duncan]L.lntraorifice sealing of gutta-percha obtumted J Endod 1998;24:659-62.
root canals to prevent coronal
29. Mah T, Basrani B, Santos JM, et al. Periapical inflammation
by white MTA orifice plugs.
30. Deveaux E, Hildelbert P, Neut C, Boniface B, Romond C. Bacterial microleakage Cavit, IRM, and TERM. Oral Surg Oral Med Oral PathoI 1992;i4:634-43. 31. Barkhordar RA, Kempler D. Microleakage of endodontic with composites.J Calif Dent Assoc 199i;25:215-8.
access cavities restored
32. Zaia M, Nakagawa R, De Quadros I, et al. An in vitro evaluation of four materials as . barriers to coronal nticroleakage
in root-filled teeth. Int EndodJ 2002;35:i29-34.
33. Webber RT, del Rio CE, Brady JM, Segall RO. Sealing quality of a temporary filling material. Oral Surg Oral Med Oral PathoI19i8;46:I23-30. 34. Beach CW, Calhoun ]C, Bramwell]D,
Hutter lW, Miller GA. Clinical evaluation of
bacterial leakage of endodontic tempomry filling materials. J Endod 1996;22:459-
treatment 35. Kazemi RB, Safavi KE, Spangberg LS. Assessment of marginal stability and perme-
K, Madison S. An evaluation of coronal microleakage treated teeth. Part 1. Time periods. J Endod 198i;13:56-9.
ability of an interim restorative endodontic material. Oral Surg Oral Med Oral Pathol
1994;i8:i8S-96. 36. Pashley EL, Tao L,Pashley DH. The sealing properties of tempomry filling materials. J Prosthet Dent 1998;60:292-i.
8. Magura ME, Kafrawy AH, Brown CE, Newton CWoHuman saliva coronal microleak-
age in obturated root canals: an in vitro study. J Endod 1991;1 i:324-31. 9. Saunders WP, Saunders EM. Coronal leakage as a cause of failure in root canal
38. Rafeek RN, Smith WA, Lalla A. Assessment of coronal microleakage
therapy: a review. Endod Dent TraumatoI1994;1O:105-8. 10. Alves J, Walton R, Drake D. Coronal leakage: endotoxin
root canals. J Endod
1995;24:5Si-91. technical quality of the root filling and the coronal 28:12-S.
use of cot-
24. Wolanek GA, Loushine RJ, Weller RN, Kimbrough WF, Volkmann KR. In vitro bac-
6. Uranga A, Blum]Y, Esver S, Parahy E, Prado C. A comparative study of four coronal obturation materials in endodontic treatment. J Endod 1999;25: 1i8-80.
11. Ray HA,Trope M. Periapical status of endodontically
23. Wolcott]F, Hicks ML, Himel yr. Evaluation of pigmented intra-orifice barriers in endodontically treated teeth. J Endod 1999;25:5S9-92.
25. Galvan RRJr, West LA,Uewehr FR, Pashley DH. Coronal microleakage
treated teeth in relation to the restoration.
Int Endod J 1995;
Balto H. An assessment of microbial coronal leakage of tempomry filling materials in endodontically treated teeth. J Endod 2002;28: i62-4. rials used in endodontically treated teeth. Eur J Prosthodont 39-43.
of three mate-
Restor Dent 2004; 12:
39. Baldissara P, Comin G, Martone F, Scotti R. Comparative study of the marginal microleakage of six cements in fixed provisional crowns. J Prosthet Dent 1998;SO: 4li-22. 40. Zmener 0, Banegas G, Pameijer CH. Coronal microleakage of three temporary restomtive materials: an in vitro study.] Endod 2004;30:582-4.
12. Hommez GM, Coppens CR, De Moor RJ. Periapical health related to the quality of coronal restorations and root Fillings. Int EndodJ 200235:6S0-9.
41. Chandler NP, Heling 1. Efficacy of three cavity liners in eliminating bacteria from
13. Tronstad L, Asbjornsen K, Doving L, Pedersen I, Eriksen HM. Influence of coronal
42. Barthel CR, Strobach A, Briedigkeit H, Gobel VB, Roulet]F. Leakage in roots coro-
restorations on the periapical health of endodontically TraumatoI2000;16:218-21. 14. Iqbal MK,Johansson
treated teeth. Endod Dent
M, Akeel RF, Bergenboltz A, Omar R. A retrospective analysis
of factors associated with the periapical status of restored, endodontically teeth.lntJ Prosthodont 2003;16:31-8.
Schwartz and Fransman
infected dentinal tubules. Quintessence Int 1995;26:655-9. nally sealed with different temporary fillings.J Endod 1999;25:i31-4. 43. Carvalho RM, Pereira JC, Yoshiyama M, Pashley DH. A review of polymerization contraction:
the influence of stress development versus stress relief. Oper Dent
1996;21:1i-24. 44. Herrera M, Castillo A, Bmvo M, UebanaJ,
Carrion P. Antibacterial activity of resin
5. Un LM, Skribner ]E, Gaengler P. Factors associated failures. J Endod 1992;18:625-i.
21. Naoum HJ, Chandler NP. Temporization for endodontics. Int EndodJ 2002;35:964-
References of endodontically
endodontic access cavities. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2002;93:il6-9.
inoculated dog teeth \vith root fillings augmented J Endod 1003;29:442- 6.
I. Schwartz RS, Robbins lW. Post placement and restoration teeth: a literature review.J Endod 2004;30:289-301.
review and treatment recom-
20. Tewari S, Tewari S. Assessment of coronal microleakage
4. The 4th generation (three step) resin adhesive systems are preferred because they provide a better bond than the adhesives that require fewer steps. 5. The "etch and rinse" adhesives are preferred to "self etching" adhesive systems if a eugenol containing sealer or temporary . material was used.
study of treated cases. Int EndodJ 2003;36:iSi-S02.
19. lIeling I, Gorfil C, Slutzky 11,Kopolovic K,Zalkind M, Slutzky-Goldberg 1.Endodontic
pulps in genn-free and conventional laboratory 1965;20:340-9.
Volume 31, Number 3, March 2005
Review adhesive:i, gJa55 ionomer and resin-modified
glass ionomer cements Md :1 com-
pOOler in contact with dentin caries samples. Oper Dent 2000;2;:26;-9.